**Electronic**

**and**

**Optical**

**Properties**

**of**

**GaAs**

**Armchair**

**Nanoribbons:**

**DFT**

**Approach**

Bramha P. Pandey

*Department of Electronics & Communication Engineering, MMMUT, Gorakhpur(U.P)‐273010. *

Received 23 August 2017; Revised 1 November 2017; Accepted 20 December 2017

**ABSTRACT**

*The electronic and optical properties of N atom‐width (N: 4, 8, 12, 16) armchair GaAs *
*nanoribbons (NA GaAs NRs) have been studied with hydrogen (H) passivated nanoribbons *
*using the DFT approach. The H passivated edge of NA GaAs NRs with different widths of *
*nanoribbons * *provide * *great * *flexibility * *to * *modulate * *the * *fundamental * *band * *gap. * *All *
*investigated width of 4, 8, 12, and 16 atom GaAs NRs are found to be semiconducting with *
*direct band gaps of 3.071, 2.275, 2.155, and 2.02 eV respectively at k‐point Z (0, 0, 0.5), *
*which exhibit interesting width dependent (N: 4~12) behaviour of the band gap. The *
*complex dielectric constant was calculated using the Kubo‐Greenwood formula, from *
*which the refractive index(n(ω)) and absorption coefficient (* *) were also calculated *
*for the bulk as well as for all width of GaAs armchair nanoribbons. The nzz* *and *
*components significantly play a major role in tuning the refractive index and optical *
*absorption coefficient of the GaAs nanoribbons. *

**Keywords** Nanoribbon(NR), Armchair, DFT, MGGA, Absorption Coefficient, Refractive
Index, Bandgap.

**1. ** **INTRODUCTION**

Two‐dimensional (2D) materials such as graphene and other variants of graphene are playing a vital and exciting role in the field of high‐speed nano devices since the last decade [1]–[3]. In particular, graphene has attracted great interest because of its unique properties; pristine graphene exhibits metallic behaviour with no band gap, whereas modified graphene can have a finite band gap. The band gap is critical to devices such as switching diodes, light emitting diodes, photodetectors, and solar cells. Different approaches have been adopted on graphene to modulate the band gap, such as graphene nanoribbon synthesis [4], bilayer control [5], [6] and chemically modified graphene[7]–[9]. However, most of these efforts have failed to achieve a significant variation in the band gap of graphene[10]. The 2D non‐graphene materials including layered, non‐layered, and the heterostructures are presently appealing and are having increased attention due to their favorable applications in electronics, optoelectronics and clean energy, and nanodevices [11], [12]. 2D non‐graphene materials are fabricated with the same efficiency and performance as graphene, which opens a new dimension for research such as the monolayer transition metal disulfide (TMD), which are likely complementary materials of graphene[13]–[17].

Recently, wavy GaAs nanoribbons were fabricated onto a strained soft substrate to investigate the strain–photonic coupling effect [18], [19]. The electronic and transmission properties of a low buckled GaAs nanoribbon have been investigated [20]. In the present work, we report the

144

first‐principle calculations of band gap modulation and optical properties such as the refractive index and the absorption coefficient in NA GaAs NRs by passivating the nanoribbon edges with a hydrogen atom using the density functional theory (DFT). In engineering, band structure, optical properties, and boundary modification of the nanoribbons are a promising and vital option. The most commonly used edge passivation is hydrogenation. The As edge of NA GaAs NRs is passivated with a hydrogen atom, which leads to the bonding of As atoms at the edges, different than the other As atoms that are bonded to Ga. Consequently, the bond length of As‐H at the edges are shorter than that in the middle of the GaAs ribbons, thus opening the energy gaps of the armchair NA GaAs NRs. The dangling bonds at the armchair edges play a vital role in governing the electronic and optical properties. The rate of the side of nanoribbon hydrogenation is determined by the temperature, pressure, and concentration of H2 in the passivation process[21]. The most favourable condition (i.e., As edges are terminated

with H) has been considered for the hydrogenation of the NA GaAs NRs. When the nanoribbon is passivated with a hydrogen atom, excess As that can be present either in elemental form or as an oxide As2O3, can be removed by the reaction mechanism[22]. The objective of this study

is to design hydrogen (H) passivated armchair GaAs nanoribbons to analyse the electronic (band gap, band structure), and optical (Refractive index, Absorption coefficient) properties of armchair GaAs nanoribbons, taking into consideration four different widths (N: 4, 8, 12, and 16) of nanoribbons.

**2. ** **COMPUTATIONALDETAILS**

The armchair GaAs nanoribbon structures can be viewed as tailoring a GaAs crystal in the (100) Miller direction with a padding of 10Å vacuum in the x and y‐direction while z is periodic and perpendicular to the armchair direction. Accordingly, the so‐called armchair GaAs nanoribbons (NA GaAs NRs) can be identified by the number of layers of atoms across the ribbon width and are labelled as NA GaAs NRs. In this work, we focus on the armchair type and shown in Figure 1, is the ball‐and‐stick model of NA GaAs NRs. We consider four different NA GaAs NRs with N = 4, 8, 12, and 16, which correspond to a width of 5.65 Å, 11.31 Å, 16.96 Å, and 22.61 Å respectively. Upon structural relaxations, the lattice constants along the periodic direction were calculated to be 4.05 Å, 3.99 Å, 3.98 Å, and 3.96 Å respectively. The atomic structure of NA GaAs NRs shows the low‐buckled honeycomb lattice structure after the relaxation of the unit cell [23].

The relaxation calculations were carried out using the first principles density functional theory (DFT) implemented in the quantum espresso source code [24]. The interaction between electrons and ions is defined by the Perdew‐Burke‐Ernzerhof (PBE) exchange‐correlation functional [25] and the ultra soft pseudopotential (USPP) [26]. The kinetic energy and charge density cut offs for the plane wave basis set were chosen at 50 Ry and 650 Ry respectively.

The energy convergence criterion for electronic and ionic iterations were set at 10‐6 _{eV and 10}‐
4_{ eV, respectively. The force convergence threshold was selected at 10}‐3_{ eV/Å in the ionic }

145 Therefore, we used the Hartwigsen, Goedecker, Hutter (HGH) pseudopotentials[30] with 4 Tier basis function for all atoms present in the unit cell. The K‐points sampling and density mesh cut off for basic functions were selected as 1x1x64 Monkhorst Pack mesh grid and 100 Ha respectively. The 1x1x128 K‐points mesh was included in the band structure and the optical spectrum calculations.

**Figure1**. Basic structure of a buckled armchair GaAs nanoribbon.

**3. ** **RESULTSANDDISCUSSION**

**3.1 ElectronicPropertiesCalculation**

146

**2a**

**Figure2aand2b.** Show the band structure of N (4, 8), and N (12, 16) armchair GaAs nanoribbons
respectively. The band structure of 4A GaAs and 8A GaAs NRs were plotted in Figure 2a with blue and
green colour respectively. Figure 2b shows the band structure of 12A GaAs and 16A GaAs NRs with blue

and green colour respectively. The calculated band structures of NA GaAs NRs predict the direct band gap nature of NA GaAs NRs at Г(gamma) and decrease as the width of GaAs nanoribbons increases.

**3.2 OpticalPropertiesCalculation**

The optical properties were calculated with the calculation susceptibility tensor, by using the Kubo‐Greenwood formula[31]. The relative dielectric constant , polarizability , and optical conductivity, , are related to the susceptibility as:

1 , , , respectively [32].

The refractive index, *n*, is related to the complex dielectric constant through

where the refractive index and extinction coefficients are *n* and *k*, respectively. The *n* and *k* are
represented in the form of real ( ) and imaginary ( ) components of the complex dielectric
constant as

and

The optical absorption coefficient is represented in the form of the extinction coefficient (*k*),

2

where the speed of light, angular frequency, and extinction coefficient are *c*, *ω*, and *k*,
respectively[33].

From the optimized structure of bulk zincblede GaAs, we calculated the refractive index, *n*(*ω*)
and optical absorption coefficient, as a function of the incident photon wavelength(*λ*)
shown in Figure 3. The calculated average values of the refractive index, *n*(*ω*) over the whole

147
range of wavelength is ~3.1(experimental 3.2 [34]) of bulk zincblende GaAs. It is noticeable
that *n(ω)* and are equal in all directions because the bulk GaAs is an isotropic and
periodic crystal. The NR GaAs NRs were optimized and the *n(ω)* and were calculated as a
function of the incident photon *λ *shown in Figure 4, 5, 6 and 7 respectively for all *N *widths (4,
8, 12, and 16). For all widths of GaAs NRs, the average refractive index is ~1.5. The *n(ω)* and

became an anisotropic crystal due to the confinement in the *x *and *y‐*direction and
periodic in the *z‐*direction. We found different values of *n(ω)* in the nxx, nyy, and nzz direction for

all four nanoribbon widths. Similarly, is the combination of all three different direction
components , for all four nanoribbon widths. It was also observed that as the
nanoribbon’s width increases from 4 to 16, the *z–* direction components become more
dominating compared with the other two components of *n(ω)* and *.* It happened because
all NA GaAs NRs are periodic in the z‐direction and had sufficient vacuum padded in the* x* and
y‐direction so that the periodic replicas of the structure cannot interact with each other. The
modulation of *n(ω)* and is possible by changing the width of NA GaAs NRs. The nzz and

components significantly play the major role in tuning the refractive index and optical absorption coefficient of the GaAs nanoribbons.

148

**Figure4.** Refractive index *n(ω)* and absorption coefficient *, *calculated with complex dielectric
constant for 4A GaAs NR.

149

**Figure6.** Refractive index *n(ω)* and absorption coefficient , calculated with complex dielectric
constant for 12A GaAs NR.

150

**4. ** **CONCLUSION**

In the present work, hydrogen (H) passivated armchair GaAs nanoribbons were designed and
the electronic and optical properties of NA GaAs NRs were calculated with the help of the DFT
theory. The modulation of the bandgap is possible by varying the width of the NA GaAs NRs as
shown in Table 1. The optical properties were calculated using the Kubo‐Greenwood formula,
from which the refractive index and absorption coefficient were calculated for the bulk as well
as for all widths of GaAs armchair nanoribbons. The refractive index *n(ω) *and the optical
absorption coefficient of the GaAs nanoribbons can be significantly modulated by varying
the widths of the GaAs nanoribbons. The most governing component of the refractive index
and optical absorption coefficient are nzz and respectively.

**Table1** Bandgap (in eV) of NA GaAs NRs with different widths (N = 4, 8, 12, 16). The band gap of bulk
GaAs has been calculated and compared with the experimental results

**Structure NA GaAs **

**NRs **

**Fundamental direct bandgap ( **

**Z-Z) **

**Experimental Bandgap **

### Bulk GaAs

### 1.41

### 1.42[35]

### 4A GaAs NR

### 3.071

### 8A GaAs NR

### 2.275

### 12A GaAs NR

### 2.155

### 16A GaAs NR

### 2.02

**ACKNOWLEDGEMENT**

The author would like to thank IUAC, Delhi and C‐DAC, Pune for providing the high‐ performance computing facility available at IUAC and C‐DAC center for this research article.

**REFERENCES**

[1] Y. Zhu, *et al.*, “Graphene and graphene oxide: Synthesis, properties, and applications,” *Adv. *

*Mater.***22**, 35 (2010) 3906.

[2] A. Splendiani, *et al.*, “Emerging photoluminescence in monolayer MoS2,” *Nano Lett.***10**, 4,
(2010) 1271.

[3] F. Bonaccorso, Z. Sun, T. Hasan, A. C. Ferrari, “Graphene Photonics and Optoelectronics,”

*Nat. Photonics***4**, 9 (2010) 611.

[4] J. Cai, *et al.*, “Atomically precise bottom‐up fabrication of graphene nanoribbons,” *Nature*,
466, 7305 (2010) 470.

[5] T. Ohta, “Controlling the Electronic Structure of Bilayer Graphene,” *Science (80)* **313**,
5789 (2006) 951.

[6] J. B. Oostinga, H. B. Heersche, X. Liu, A. F. Morpurgo, L. M. K. Vandersypen, “Gate‐induced
insulating state in bilayer graphene devices,” *Nat. Mater.***7**, 2 (2008) 151.

[7] X. Dong, *et al.*, “Symmetry breaking of graphene monolayers by molecular decoration,”

*Phys. Rev. Lett.***102**, 13 (2009).

[8] K. Novoselov, V. Fal, L. Colombo, “A roadmap for graphene,” *Nature*, **490**, 7419 (2012)
192.

151 [10] K. Kim, J.‐Y. Choi, T. Kim, S.‐H. Cho, H.‐J. Chung, “A role for graphene in silicon‐based

semiconductor devices.,” *Nature*, **479**, 7373 (2011) 338.

[11] F. Wang, *et al.*, “Synthesis, properties and applications of 2D non‐graphene materials,”

*Nanotechnology*, **26**, 29 (2015) 292001.

[12] B. Santhibhushan, M. Soni, A. Srivastava, “Optical properties of boron‐group (V)
hexagonal nanowires: DFT investigation,” *Pramana – J. Phys.***89 (2017) 14. **

[13] S. Das, H. Y. Chen, A. V. Penumatcha, J. Appenzeller, “High performance multilayer MoS2
transistors with scandium contacts,” *Nano Lett.* 1**3**, 1, 92013)100.

[14] W. Zhang, *et al.*, “Ultrahigh‐gain photodetectors based on atomically thin graphene‐MoS2
heterostructures.,” *Sci. Rep.***4** (2014)3826.

[15] M. Bernardi, M. Palummo, J. C. Grossman, “Extraordinary sunlight absorption and one
nanometer thick photovoltaics using two‐dimensional monolayer materials,” *Nano Lett.*

**13**, 8 (2013) 3664.

[16] T. Roy, *et * *al.*, “Field‐effect transistors built from all two‐dimensional material
components,” *ACS Nano***8**, 6 (2014) 6259.

[17] B. Radisavljevic, A. Kis, “Mobility engineering and a metal‐insulator transition in
monolayer MoS₂.,” *Nat. Mater.***12**, 9, (2013) 815.

[18] Y. Wang, *et al.*, “Buckling‐Based Method for Measuring the Strain–Photonic Coupling
Effect of GaAs Nanoribbons,” *ACS Nano***10**, 9 (2016) 8199.

[19] C. Sealy, “GaAs nanoribbons take the strain,” *Nano Today***11**, 5 (2016) 539.

[20] B. P. Pandey, “Electronic and Transmission Properties of Low Buckled GaAs Armchair
Nanoribbons,” *J. Surf. Sci. Technol.***33**, 3 (2017) 91.

[21] B. Mahler, V. Hoepfner, K. Liao, G. A. Ozin, “Colloidal synthesis of 1T‐WS2 and 2H‐WS2
nanosheets: Applications for photocatalytic hydrogen evolution,” *J. Am. Chem. Soc*. **136**,
40 (2014) 14121.

[22] A. A. Balmashnov, K. S. Golovanivsky, E. M. Omeljanovsky, A. V Pakhomov, A. Y. Polyakov, “Passivation of GaAs by atomic hydrogen flow produced by the crossed beams method,”

*Semicond. Sci. Technol.***5** (1990) 242.

[23] H. Şahin *et al.*, “Monolayer honeycomb structures of group‐IV elements and III‐V binary
compounds: First‐principles calculations,” *Phys. Rev. B ‐ Condens. Matter Mater. Phys.***80**,
15 (2009).

[24] P. Giannozzi *et al.*, “QUANTUM ESPRESSO: a modular and open‐source software project
for quantum simulations of materials.,” *J. Phys. Condens. Matter***21**, 39 (2009) 395502.
[25] J. Perdew, K. Burke, Y. Wang, “Generalized gradient approximation for the exchange‐

correlation hole of a many‐electron system,” *Phys. Rev. B***54**, 23 (1996) 16533.

[26] K. Laasonen, R. Car, C. Lee, and D. Vanderbilt, “Implementation of ultrasoft
pseudopotentials in ab initio molecular dynamics,” *Phys. Rev. B***43**, 8 (1991) 6796.

[27] H. J. Monkhorst, J. D. Pack, “Special points for Brillouin‐zone integrations,” *Phys. Rev. B***13**,
12 (1976) 5188.

[28] “Atomistix ToolKit version 2016, 2, QuantumWise A/S (www.quantumwise.com).

[29] F. Tran, P. Blaha, “Accurate Band Gaps of Semiconductors and Insulators with a Semilocal
Exchange‐Correlation Potential,” *Phys. Rev. Lett.***102 (2009) 226401. **

[30] C. Hartwigsen, S. Goedecker, J. Hutter, “Relativistic separable dual‐space Gaussian
pseudopotentials from H to Rn,” *Phys. Rev. B***58** (1998) 3641.

[31] W. A. Harrison, *Solid state theory*. New York: McGraw‐Hill, 1970.

[32] R. M. Martin, “Electronic Structure: Basic Theory and Practical Methods,” *Book*. (2004)
624.

[33] D. J. Griffiths, *Introduction to Electrodynamics*, 3rd ed. New Jersey: Prentice Hall, 1999.
[34] B. Herrmann, *Synthetic Methods of Organometallic and Inorganic Chemistry*, 2nd ed. New

York: Georg Thieme Verlag Stuttgart, 1996.